- Email: [email protected]

Contents lists available at ScienceDirect

Chemical Engineering Journal journal homepage: www.elsevier.com/locate/cej

Impact of washcoat distribution on the catalytic performance of gasoline particulate filters as predicted by lattice Boltzmann simulations Igor Belot a, David Vidal a, b, *, Robert Greiner c, Martin Votsmeier c, d, Robert E. Hayes e, François Bertrand a, * a

Research Center for Industrial Flow Processes (URPEI), Department of Chemical Engineering, Polytechnique Montr´eal, Montr´eal, QC H3C 3A7, Canada Department of Mechanical Engineering, Polytechnique Montr´eal, Montr´eal, QC H3C 3A7, Canada UMICORE AG & Co. KG, Rodenbacher Chausee 4, 63457 Hanau, Germany d Technische Universit¨ at Darmstadt, Ernst-Berl-Institut für Technische und Makromolekulare Chemie, Alarich-Weiss-Straße 8, 64287 Darmstadt, Germany e Department of Chemical and Material Engineering, University of Alberta, Edmonton, AB T6G 2G6, Canada b c

A R T I C L E I N F O

A B S T R A C T

Keywords: Catalyst-coated particulate filter Washcoat uniformity Catalytic conversion Coating effectiveness Porous media Lattice Boltzmann method

The impact of catalyst distribution within the porous wall of a coated gasoline particulate filter on its catalytic performance is investigated. Sections of catalyzed filter wall with different amounts of washcoat and different levels of uniformity are digitally reconstructed from tomography data. A coupled problem involving the exhaust gas flow and the transport and reaction of a dilute species in the reconstructed structures is solved using the lattice Boltzmann method. The resulting model is verified and its accuracy is assessed for first-order reactions and those with inhibition kinetics. Computed washcoat effectiveness values agree well with the Thiele modulus theory. Improvements in catalytic conversion and washcoat effectiveness of uniform washcoat distribution are observed with increased washcoat loading. These effects are quantified and the benefits are found to be limited to the transitional regime. The uniform washcoat distribution is shown to be beneficial for both filtration and conversion performance.

1. Introduction A World Health Organization survey reported an alarming 3 million deaths in 2016 due to poor air quality [1]. Part of this air pollution is caused by the exhaust gases of internal combustion engines of heavy and light duty vehicles [2]. To reduce the negative impact of the trans portation sector on air quality, manufacturers have added two devices to the exhaust gas aftertreatment system of modern vehicles. The first is the particulate filter (PF), which is customarily used for diesel vehicles (known as DPF for diesel particulate filter), but has recently been introduced to the gasoline direct injection (GDI) vehicle market (known as GPF for gasoline particulate filter) [3]. It is aimed at capturing fine soot particles resulting from the incomplete burning of fuel in the engine combustion chamber that are carried in the exhaust gas. The second device is the catalytic converter (CC), which can be placed upstream and/or downstream from the PF. It is aimed at converting pollutants that are threats to human health and the environment such as carbon mon oxide (CO), nitrogen oxides (NOX), and hydrocarbons (HC) into benign

gaseous products such as CO2, N2 and H2O. There are different types of catalytic converters depending on the type of vehicle and the gases that have to be treated. Both the PF and the CC are honeycomb monoliths with typically square 1–2-mm-wide channels. In the case of the PF, the channels are alternatively plugged at the inlet or the outlet to force the exhaust gas to pass through the porous wall separating them. The fine particles carried by the gas flow are captured when they collide with the solid structure of the porous wall through electrostatic interactions. In the CC, the gas simply travels along the catalyst-coated channels such that the pollutants diffuse and react in the catalyst coating when passing through the device [4]. In recent years, manufacturers have developed catalyst-coated PFs (CPF) by depositing catalyst coating, called washcoat, within the porous wall of the PF to create a single device that combines the catalytic conversion and filtration functionalities. This multifunctional device has the advantage of being more compact and less costly, easing heat up during a vehicle cold start, lowering the overall pressure drop of the exhaust gas aftertreatment system, and easing soot combustion [5]. At the reactor scale, it also facilitates contact between the catalyst coating and the

* Corresponding authors at: Research Center for Industrial Flow Processes (URPEI), Department of Chemical Engineering, Polytechnique Montr´ eal, Montr´ eal, QC H3C 3A7, Canada (D. Vidal). E-mail addresses: [email protected] (D. Vidal), [email protected] (F. Bertrand). https://doi.org/10.1016/j.cej.2020.127040 Received 20 May 2020; Received in revised form 28 August 2020; Accepted 13 September 2020 Available online 19 September 2020 1385-8947/© 2020 Elsevier B.V. All rights reserved.

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

temperatures [16-19]. An experimental comparison of numerous cata lyst configurations within the porous wall of a PF in terms of filtration and catalytic conversion performance showed that the best configura tion is a filter with an SiC filtration membrane coated with a catalyst layer [20]. In addition, experimental testing of different coating loca tions within the porous walls of a GPF showed that an in-wall coating improves the catalytic performance of the TWC whereas an on-wall coating improves the filtration efficiency of the c-GPF [21]. Other experimental studies on the impact of washcoat distribution on the performance of CPFs can be found in the literature [12,22,23]. The general conclusion is that a catalyst coating of a PF results in higher filtration performance but lower catalytic performance than a sequential treatment through a CC and a PF. This can be partly explained by (1) the reduction in the pore space, leading to better capture efficiency in general, and (2) the mass transfer limitation in a wall-flow configuration of a CPF [24]. Overall, these studies did not precisely characterize the washcoats tested, and a limited number of cases were investigated. Numerically, several methods have been reported in the literature to evaluate the filtration and catalytic performance of a CPF. Although the multiscale nature of these systems offers a wide range of possibilities for researchers to develop predictable models, they are faced with numerous difficulties. All the different scales of CPF modelling, namely the whole filter scale, the channel scale, and the porous wall scale, as illustrated in Fig. 1 of [25], have been presented in a number of exhaustive reviews [4,26,27]. The whole device scale is often used to investigate the conversion performance of a classical catalytic monolith converter [4,28] or the energy and filtration performance of a PF [29], but is not suited to investigate the impact of washcoat distribution on the overall performance of a CPF. At the channel scale, numerous 1D or 2D models have been developed over the years. For the prediction of cat alytic performance, [30] developed a 1D model to assess the oxidation of soot and NOX using experimental data for the calibration of kinetic pa rameters. [31] presented a 1D porous medium approach that represents a SCR-DPF as a continuum medium. [23] proposed a channel scale model to predict ΔP, filtration, soot oxidation and ash effects. These models are based on balance equations for mass, momentum, and energy in two adjacent channels of the PF [32-35]. The advantage of such volume-averaged models is the low computational cost while their main drawback remains the tuning of parameters using other smaller scale models or experiments. Still, these models can be useful for providing general trends for optimizing the global parameters of a CPF, as was done in a recent study for catalyst zoning in a c-DPF [36]. However, channel scale models are not precise enough to reveal the impact of washcoat distribution within the porous wall on the performance of the filter. At the microscopic scale, the main difficulties in modelling the conversion of pollutants in a CPF are the large number of species and concurrent reactions [37] in combination with the complexity of the catalyst and substrate structures involved. To overcome these diffi culties, simplified reaction models have been introduced for SCR-DFP that replace the solution of partial differential equations (PDEs) with a closed-form solution. The basic rules of these models, which are known as kinetics splitting schemes, have been described in an exhaustive re view [38]. However, in a recent study, it was shown that these volumeaveraged models usually overestimate the conversion performance of CPFs by not considering transport limitations. This has been under scored by a recent 3D study at the pore scale [24]. New 1D models have thus been proposed that take these limitations into consideration and that show very good agreement with 3D simulations at the wall scale. To fully understand the impact of a catalyst coating on the performance of a CPF and to feed larger-scale model inputs, simulations that directly solve partial differential equations at the microscale are needed. The meth odology used by such models is usually multi-step and makes it possible to predict the filtration or catalytic performance of the CPF. The first step involves the reconstruction a representative elementary volume (REV) of the porous structure of the CPF. This can be done using

Nomenclature ADR BW CC CPF DPF FDM FEM FVM GDI GPF LBM N1-N8 NS OS PF REV SCR TWC U1-U4

Advection-diffusion–reaction Bare wall Catalytic converter Catalyst-coated particulate filter Diesel particulate filter Finite difference method Finite element method Finite volume method Gasoline direct injection Gasoline particulate filter Lattice Boltzmann method Structure series with a non-uniform washcoat distribution Navier-Stokes Original sample Particulate filter Representative elementary volume Selective catalytic reduction Three-way catalyst Structure series with a uniform washcoat distribution

chemical species through the advection of the exhaust gas into the tortuous porous wall as opposed to the simple gas diffusion that takes place in a classical CC reactor [6]. For diesel engine applications, the selective catalytic reduction (SCR) functionality is usually integrated into the PF [7,8]. For GDI engine applications, the three-way catalyst (TWC) functionality is now more often integrated into the PF [5]. TWC is designed to handle simultaneously the three aforementioned pollutants (NOX, CO, HC) using oxidation and reduction reactions [9]. The TWC coating consists of a porous material containing the precious group metals platinum, palladium and rhodium [8,10,11], which need to be used sparingly for cost reasons. The efficiency of CPFs is very promising, as a single SCR-DPF displays the same deNOX efficiency as two SCR-CC systems in series [12]. However, even if the combination of these two aftertreatment devices (i.e., PF and CC) is expected to achieve an almost equivalent performance as the two separate units, the performance is not guaranteed and can certainly be optimized. Indeed, the distribution uniformity and the amount of catalyst deposited within the porous space of the PF can alter its pore size distribution [13]. This can have a sig nificant impact on its overall performance characterized by (1) its pressure drop (∆P), (2) its filter efficiency (Ef), and (3) its catalytic conversion (X), with the objective being to have the highest X and Ef at the lowest possible ΔP. To gain a better understanding of the impact of washcoat distribution on the performance of a CPF, numerous recent studies have endeavored to evaluate the filtration and catalytic performance of different CPF configurations. In the context of a coated diesel particulate filter (cDPF), an experimental study proposed to find the optimal CuFe2O4based catalyst load in the PF to lower ΔP and the soot oxidation tem perature at the same time using scanning electron microscopy (SEM), energy dispersive spectroscopy (EDAX), mercury porosimetry, TG-DTA analysis, H2-TPR measurements, and bending strength tests [14]. Another study experimentally underscored the importance of wallsurface coating location in the channels of the PF, specifically by comparing depositions at the inlet and at the outlet of the channel wall of a SCR-DPF and by measuring ΔP and NOX conversion using an FTIR spectrometer [15]. The results showed that, in a diesel context, the impact of soot accumulation surpasses the impact of washcoat distri bution and location on CPF performance. In the context of a coated gasoline particulate filter (c-GPF), soot accumulation is expected to have a minor impact due to lower particle concentrations and higher gas 2

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

Fig. 1. Illustration of the three-step numerical model used to predict the catalytic performance of a c-GPF porous wall at the microscopic scale level.

geometrical reconstructions such as spherical particle packing algo rithms [39,40], stochastic techniques such as simulated annealing [41], real sample images such as SEM images [42], or computed tomography scans [43]. The second step is to calculate the flow field through the pore space by solving the Navier-Stokes (NS) equations. For this purpose, several CFD methods can be employed, including the well-known finite volume (FVM), finite element (FEM) and lattice Boltzmann methods (LBM). The last step is to calculate the capture efficiency or chemical conversion of the CPF by solving the Langevin equation for every soot particle or an advection–diffusion-reaction (ADR) equation for the soot and/or chemical species concentrations. [44-48] used a three-step methodology to (1) reconstruct the porous wall using tomographic im ages of real CPFs or washcoat depositions, (2) compute the flow field with FVM using open source OpenFOAM® software, and (3) solve the ADR equation in the porous medium using another in-house FVM solver. Similarly, in a previous study, the filtration performance of a series of REV of a c-GPF for various washcoat amounts and uniformity degrees was investigated with a 3D wall-scale model using LBM [25]. For the operating conditions and substrate investigated, it was found that, for the same amount of washcoat, a uniform washcoat distribution profile results in a higher capture of soot particles than a non-uniform distri bution, partly due to flow channeling effects that deteriorate filtration efficiency in the latter case. In [49], a non-isothermal model of a channel of a c-DPF developed using open source OpenFOAM® software showed that isothermal models are adequate for representing these systems. [5052] used LBM to develop a model to predict soot filtration as well as soot and NOX oxidation by the platinum catalyst within the catalyst-coated DPF. They investigated where the reactions take place to better under stand the evolution of the NO/NO2 ratio in the thickness of the porous PF wall. Lastly, an even smaller scale can also be considered. This is the pore scale of the catalyst itself as it is a porous material. Simulations of dif fusion–reaction processes have been conducted using ANSYS FLUENT® software by [53] at the scale of the washcoat microstructure obtained from focused ion beam scanning electron microscope images of a rhodium alumina catalyst-coated monolith. They predicted catalyst

performance as a function of the pore-scale microstructure and quanti fied pore effectiveness and reaction–diffusion limitations as a function of ¨hler number. Simulations at this scale can thus be used, for the Damko example, to retrieve effective diffusion coefficients of chemical species in the catalyst coating. Various numerical methods, including FVM, LBM, and FDM, have been used in the context of CPF to solve the NS and ADR equations at the microscale. Of these, the LBM has been reported to be more accurate than classical FDM schemes (explicit Euler and implicit Crank-Nicolson) for advection-dominated mass transport problems [54] and makes possible larger time steps for the same space discretization [55]. Although the feasibility of building predictable and relevant micro scale models is possible, to the authors’ knowledge, no study on the impact of the distribution of the catalyst in the porous space of the CPF walls on both its filtration and catalytic performance has ever been conducted. [25] recently numerically studied such an impact on filtra tion performance for a cordierite substrate of a GPF. It would thus be natural to extend this study to catalytic performance. In this context, and following on from [25], the objective of the present study was to eval uate the impact of uniform and non-uniform washcoat distributions and amounts in the porous wall of a c-GPF on catalytic performance. Together with the filtration performance reported in [25], a comparison between uniform and non-uniform washcoat distributions in terms of overall performance was then carried out. The remainder of this paper is organized as follows. In Section 2, the three-step numerical model developed to study the impact of washcoat amount and uniformity on the catalytic performance of a c-GPF is detailed. In Section 3, the catalytic performance results for 14 recon structed porous wall structures presenting two different degrees of catalyst distribution uniformity with several amounts of catalyst are presented both in terms of conversion and catalyst coating effectiveness. An example of how the proposed approach can be used to provide guidance in improving washcoat deposition is then provided. Lastly, Section 4 provides concluding remarks and guidelines for improving washcoat distribution in a c-GPF and for extending this work in future investigations. 3

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

Fig. 2. Close-up cross-sectional 200 × 100-pixel visualizations (with dx = 1.25 µm) for each of the 14 structures reconstructed in [25] and investigated in the present study, i.e., the non-uniform series (N1-N8) containing the original R&D sample (OS), the uniform series (U1-U4), and the bare wall (BW) structures.

and the pore space must be accurately digitally retrieved. For this purpose, a computed tomography (CT) scan of a 3 × 3 × 1.5mm3 piece of a 1.16-mm-wide channel of a c-GPF was acquired using a General Electric Phoenix Nanotom M apparatus, the preparation of which is detailed in [24]. A rectangular cuboidal 256 × 801 × 779-voxel domain of cordierite wall covered with a TWC washcoat was extracted from this scan and is depicted in Fig. 3 of [25]. This 8-bit grey scale image was segmented to distinguish between the washcoat, cordierite and pore space phases using the MATLAB Image Processing Toolbox™. The voxel resolution of this domain in every direction imposed by the digital resolution of the CT scanner was dx = 1.25 μm. As a result, the thickness of the wall, from side to side, is L = 256 × dx = 320 μm. Moreover, the mean pore diameter being ~ 30 µm in such structures, the average number of voxels in a pore diameter is 24, which is sufficient to accurately compute the flow as shown in [56]. This cuboidal domain is referred to as the original R&D sample (labelled OS). In this OS struc ture, the catalyst is non-uniformly distributed within the cordierite porous structure, due to the deposition process that involves capillary/ wettability effects, that may lead to occlusion of pores entrance, pre venting the spread of the catalyst inside the pores. From this OS struc ture, two series of structures presenting two different catalyst distributions were created using a set of morphological image processing operations applied on the segmented X-ray computed tomography data, as proposed by [25]. This resulted in a non-uniform washcoat distribu tion series consisting of 9 structures with increasing amounts of catalyst labelled N1 to N8, as well as the OS structure, and a uniform washcoat distribution series consisting of 4 structures with increasing amounts of catalyst labelled U1 to U4. A bare wall (BW) structure presenting no catalyst deposition was added to these 13 structures, bringing the total number of structures studied to 14. For ease of computation, each of these 14 structures was partitioned into four 256 × 389 × 400-voxel subdomains, the size of which is an REV of the porous wall described in [25]. This is illustrated in Fig. 3 in [25]. This last operation brought the number of reconstructed subdomains to 56. More details on the set of morphological image processing operations employed to deposit washcoat artificially within the cordierite structure (BW) are given in [25]. A 200 × 100-pixel cross-sectional visualization of each of the 14 structures investigated in the present study is presented in Fig. 2. For the numerical study presented herein, the three phases of the structures were encoded as follows: 0 for the pore space, 1 for the cordierite, and 2 for the catalyst phase. The volume fraction of phase i is denoted as ϕi . For the combined solid phase (catalyst + substrate), ϕ1+2

2. Three-step methodology To predict the catalytic performance of a c-GPF at the microscale and compare washcoat distribution uniformities within its porous wall, a three-step methodology was developed. It consisted of (1) numerically reconstructing a representative elementary volume (REV) of the GPF porous wall coated with a uniform or a non-uniform catalyst deposition with several amounts of washcoat, (2) computing the flow field, and (3) computing the concentration field of a hypothetical chemical species carried by the flow through the previously reconstructed porous wall structures by solving a one-way coupled problem involving the NavierStokes (NS) equations and an advection–diffusion-reaction (ADR) equation using the lattice Boltzmann method (LBM). This procedure is illustrated in Fig. 1. Given the large number of chemical species and the concurrent re actions that take place in a c-GPF, evaluating the catalytic performance in a comprehensive way would require solving as many ADR equations throughout the domain as there are chemical species involved in those reactions. To reduce the computational load and considering that the goal here was to determine whether or not the catalyst is optimally distributed throughout the structure for a given washcoat deposition, a single first-order reaction of a hypothetical chemical species was mainly considered. Furthermore, it must be mentioned that this three-step methodology is in fact part of a four-step methodology that can pre dict the overall performance of a c-GPF at the microscale involving both filtration and catalytic conversion aspects. The additional step of this methodology, which involves the prediction of filtration efficiency, is presented in [25] as are steps (1) and (2), which are also necessary for computing filtration efficiency. In this section, step (1) is first recalled, then the LBM used in steps (2) and (3) is presented in detail. This is followed by a description of the computational and physical assump tions that were used. 2.1. Porous wall reconstruction and characterization To predict the catalytic performance of a c-GPF at the wall scale, the first step is to reconstruct a representative elementary volume (REV) of the porous wall that separates adjacent channels within the c-GPF monolith and that is taken here as the smallest volume over which the permeability measured is representative of the whole porous wall (see [25]). The accuracy of the prediction of the catalytic performance of the system is highly dependent on the accuracy of the reconstruction of the structure. For example, the interfacial surface area between the catalyst 4

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

areas Si,j were calculated using a statistical method described in [57] and corrected by a factor 23 to account for the inherent surface area overestimation due to the staircase-like fractal nature of a voxelized sur face representation, as pointed out in the literature [58,59]. This prop erty is a critical metric for the catalytic and filtration performance of a cGPF. For overall c-GPF performance, it is generally beneficial to maxi mize (1) the surface area of the catalyst with respect to the pore space for chemical reactions, and (2) the surface area of the whole solid phase with respect to pore space for soot capture. A characteristic length for the catalyst phase, which can be inter preted as the average thickness of the catalyst deposition, can then be defined by: Lcat =

ϕ2 fw εBW Vcat = = S0,2,0 S0,2,0 S2,0

(3)

where S0,2,0 is the surface area between the pore space and the catalyst phase per unit volume of porous medium, and Vcat is the volume of the catalyst phase. The surface area of the solid phase S0,(1+2),0 is also linked to the mean pore diameter, denoted dw , as in [60]: dw =

2ε 6 3 S0,(1+2),0

(4)

The geometrical descriptors listed above serve two purposes. The first is to understand better the causal relation between the geometrical parameters of the reconstructed porous structures and catalytic perfor mance. The second is to allow other researchers to replicate these ex periments. Additional geometrical descriptors calculated on the structures generated for the present study can be found in [25]. 2.2. The lattice Boltzmann method In the context of porous media, the lattice Boltzmann method (LBM) has received increasing attention from researchers over the last two decades because of its ease of implementation, its great potential for parallelization [61,62] and its ability to deal with complex geometries [56]. It is not only a CFD solver but also a partial differential equation (PDE) solver [55]. It is thus possible to solve both the NS and ADR equations in a coupled way using the same overall numerical scheme. Although the LBM is intrinsically a transient PDE solver that can be used to study the response to temporal fluctuations in concentration, only the steady-state solutions resulting from steady boundary conditions are analyzed here. For these reasons, the LBM is particularly well adapted to the prediction of catalytic performance in porous media. It consists of solving any PDE using the Boltzmann equation from the kinetic theory of gases given by:

Fig. 3. D3Q15 (top) and D3Q7 (bottom) velocity vector sets used for the dis cretization of the microscopic velocity domain, respectively, in flow and mass transport problems.

∂f + e.∇x f + F.∇e f = Ω(f ) ∂t

where Ω is an appropriate collision operator and f represents a probability distribution function of finding a quantity of interest or “population” traveling at a microscopic velocity e, being at position x at time t, and being driven by an external force F. Although derived from the kinetic theory of gases, this equation, which was originally used to describe the micro-dynamical evolution of a population of molecules in a gas, can also be used to evolve any given population (e.g. populations of molecules in a liquid, quanta of energy, a chemical species in a me dium) and thus model any transport phenomena. To solve this equation, the discretizations of the partial derivatives in space and time are carried out by the voxelization of the domain (in which phases are eventually encoded in a Boolean manner) using a Cartesian grid (also called lattice) and by a classic Euler explicit scheme, respectively. The discretization of the microscopic velocity domain is accom plished by projecting the distribution functions on a set of discrete ve locities ei denoted by DnQm, where n is the number of spatial dimensions and m the number of discrete velocities used. The sets of velocities used

is simply denoted as ϕ and is commonly referred to as the solidity. For the porous phase, ϕ0 is denoted ε and is thus commonly referred to as the porosity. Having the porosity of the reconstructed structures, the frac tion of pore volume filled by the catalyst can be calculated as: fw = 1 −

ε εBW

(1)

where εBW is the porosity of the BW structure. This descriptor is representative of the amount of washcoat introduced into the BW sub strate and will be used to report the results in Section 3. The surface area between phases i and j per unit volume of porous medium can be defined as: S0,i,j =

Si,j Vtot

(5)

(2)

where Si,j is the interfacial area between phase i and j, and Vtot is the bulk volume of the porous medium. In the present study, the surface 5

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

in the present study were D3Q15 and D3Q7 for solving the NS and ADR problems, respectively, as shown in Fig. 3. In the case of an ADR problem involving isotropic diffusion with zero off-diagonal coefficients and a linear behavior, a simpler set of microscopic velocities such as D3Q7 as well as simpler equilibrium functions have been found to be sufficient to solve such phenomena [55,63]. In this work, the LBM was employed to compute the flow field through the reconstructed porous wall structures using the second-order accurate computer code developed in [61,62] as well as the concentration field using a custom-written program devel oped specifically for the present study. Assuming that the low concen tration of the chemical species does not affect the gas flow field, a oneway coupling of these two solvers was used to evaluate the catalytic performance of the c-GPF. First, the flow field was solved and the flow properties through the structure were obtained. Then, taking the pre viously computed flow field as input data, the mass transport of a hy pothetical dilute species was solved to obtain its concentration field throughout the domain. From this, the catalytic performance of the structures was obtained. Details about the LBM schemes used for solving both the NS and ADR equations are provided in the following sub sections to make it possible to compare the implementations. For addi tional information about the LBM, the reader is referred to the studies by [55,64].

∑ fi (x, t) i ∑ ρu(x, t) = ei fi (x, t)

ρ(x, t) =

Lastly, to enforce the quasi-incompressibility and to obtain the pressure field p, the following equation of state is used [66]: ( ) ) ‖ΔP‖ ( p(x, t) = ρ(x, t) − ρ(x, t) c2s − xf − L L

2.2.2. Concentration field computation To compute the concentration field of a dilute chemical species, the most common procedure consists of solving the ADR equation. For a chemical species in a specific medium and a constant diffusion coeffi cient D, it reads as:

(6)

where Fi is an external body force and fi represents here populations of the exhaust gas molecules (assumed here to be air as a first approxi mation) with microscopic velocity ei (with i ∈ {0, 1, 2, 3, 4, 5, 6, 7, 8, 9, 10, 11, 12, 13, 14} propagating at every time step dt from a lattice node to its nearest neighbor in the direction of the microscopic velocity. The collision operator Ωi is approximated using a single relaxation procedure toward a local equilibrium state proposed by Bhatnager-Gross-Krook [65], which is commonly used due to its simplicity and accuracy. It reads as: Ωi (x, t) = −

1

τf

eq

(fi (x, t) − fi (u, ρ) )

∂c + u∙∇c = D∇2 c + r ∂t

(13)

where c is the concentration of the chemical species and r is a re action rate. Instead of directly solving the ADR equation, as for the NS equations, the LBM solves a discretized Boltzmann equation in time, space, and velocity domains ei , i ∈ {0, 1, 2, 3, 4, 5, 6}, which reads as: gi (x + ei dt, t + dt) = gi (x, t) + Ω’i (x, t) + γ i r

(14)

where gi is used here to represent the corresponding populations of the dilute gas species and distinguish them from the air gas molecule populations fi . They thus represent populations of the chemical species propagating at velocity ei along the lattice and colliding according to:

(7)

where τf is a dimensionless relaxation time (here, τf = 1 is used for accuracy reasons [61,69]). In addition, according to the kinetic theory of gases, the equilibrium population fi eq follows a Maxwell-Boltzmann distribution that can be approximated by a second-order expansion in velocity such that: ( ) ei ∙u (ei ∙u)2 u∙u eq fi (u, ρ) ≈ ωi ρ 1 + 2 + (8) − cs 2c2s 2c4s

Ω’i (x, t) = −

1

τg

(gi (x, t) − gi eq (u, c) )

(15)

in which τg is the dimensionless relaxation time towards an equi librium state represented by gi eq defined as: ) ( ei .u gi eq (u, c) = γi c 1 + 2 (16) cs

which depends on the local macroscopic fluid velocity u = u(x, t) and density ρ = ρ(x, t), where ωi is a weight associated with velocity ei (with 1 ω0 = 29; ω1− 6 = 19; ω7− 14 = 72 ) and cs represents the speed of sound in the lattice space defined by: dx cs = √̅̅̅ 3dt

(12)

for 0 ≤ xf ≤ L, where xf and L are, respectively, the position and the domain thickness in the direction of the flow and ΔP is the pressure drop through the filter thickness. The second term on the right-hand side of Eq. (12) represents the static pressure that needs to be added when periodic boundary conditions applied to the populations combined with a body force are used to impose a ΔP through the thickness, as is the case in this study. This body force is added as a source term in the right-hand side of the LBM scheme (i.e., Eq. (6)) (see [66]). For the flow calculation, only two phases are considered: the solid phase (cordierite + washcoat) and the fluid phase (pore space). Once calculated, being strictly in a laminar regime, the flow field can be rescaled a posteriori to match the actual targeted superficial velocity U, and the ΔP is then rescaled accordingly.

2.2.1. Flow field computation Instead of directly solving the NS equations, the LBM solves a dis cretized Boltzmann equation in the time, space, and velocity domains, and reads as: fi (x + ei dt, t + dt) = fi (x, t) + Ωi (x, t) + Fi

(11)

i

where u and c are, respectively, the macroscopic velocity and the concentration of the chemical species, and γi is the weight related to the velocity ei (γ 0 = 14; γ1− 6 = 18). As for the flow calculation, cs represents the speed of sound in the lattice space as expressed by Eq. (9). The time step dt, the diffusion coefficient of the species D, and the dimensionless relaxation time τg are related through the following equation: ( ) 1 (17) D = c2s dt τg − 2

(9)

where dx is the lattice spacing. The dimensionless relaxation time is related to the fluid kinematic viscosity ν through: ) ( 1 (10) ν = c2s dt τf − 2

The value of the time step dt and, as a result, that of cs are different from those in the flow simulation. It would eventually be possible to adjust the relaxation time of an LBM solver so that the time steps used by the NS and ADR LBM solvers are equal. In any case, as there is a one-way coupling between the two codes, this is not necessary here and has no influence on the results. Summing all the populations gi , it is possible to

Summing zeroth- and first-order moments of the populations fi , the macroscopic fluid properties ρ and u at every position and time can be retrieved by:

6

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

retrieve the macroscopic physical value of c at every position and time as in [55]: ) ( ∑ 1 r(x, t) (18) c(x, t) = gi (x, t) + 1 − 2τg i

Table 1 Physical parameters used in the calculations of the flow and concentration fields with the LBM, considering air as a carrying fluid and a hypothetical chemical species. Parameter

A first-order reaction was considered in the present study to follow a classical textbook approach [67,75]. It is expressed as r(x, t) = − k1 c(x, t), where k1 is the rate constant. It made it possible to compare the catalytic performance of the two distribution profiles investigated. However, to extend the results presented in Section 3 to more realistic reaction rates, an inhibition kinetics (LHHW type) was also considered [68]. It can be expressed as r(x, t) = −

k1 c(x,t) , (1+Kc(x,t))2

− 3

Fluid density (kg.m ) Fluid dynamic viscosity (kg.m− 1.s− 1) Superficial velocity (m.s− 1) Temperature (K) Diffusion coefficient in pores (m2.s− 1) Effective diffusion coefficient in catalyst (m2.s− 1) First-order reaction rate constant (s− 1) Inhibition kinetics constant (m3/mol) Inlet concentration (mol/m3)

where k1 and K are the kinetics and

inhibition constants, respectively.

2.2.3. Boundary conditions For the flow simulations, 100-voxel buffers were added at the inlet and outlet in the flow direction (x) of the structures studied, resulting in 456 × 400 × 389-voxel computational domains. This aimed to facilitate the imposition of the periodic boundary conditions in the flow direction and to avoid an boundary effect at the entrance of the porous structure. For the ADR simulations, 20-voxel buffers were added at the inlet and outlet in the flow direction (x), resulting in 296 × 400 × 389-voxel computational domains. Contrary to other classical methods, boundary conditions for the LBM are not applied directly on the macroscopic values but on the microscopic populations fi or gi instead. For the computation of the flow field, periodic boundary conditions were applied in the flow direction (x), and symmetric boundary conditions were applied in the directions perpendicular to the flow (y,z) at the outer domain boundaries. As previously mentioned, the periodic boundary conditions combined with a body force were used as a classical way to impose a ΔP through the thickness direction (x) [55,66]. At the interface between the fluid and solid voxels, a half-way bounce-back boundary condition was applied to make the solid phase impermeable to the flow. More details on the implementation and the characteristics of these boundary conditions can be found in [61,62]. For the concentration field at the inlet (x = 0), a Dirichlet boundary condition in concentration, c = c0, was applied, which translates at the microscopic scale into: ∑ g1 (x, t + dt) = c0 − gi (x, t + dt) (19)

Value

ρ

0.543 3.18 × 10-5 0.055 650 6.50 × 10-5 10-6 1.05 × 104 2 1

µ U T Dpor Dcat k1 K c0

to the hypothetical chemical species considered, similar to Eq. (21). At the pore-catalyst interface, no specific boundary condition was applied, but the diffusion coefficient was different across the interface: Dcat and Dpor for the catalyst and pore phases, respectively. The choice of τg,por = 1, for accuracy reasons [61,69], led to the two following dimensionless relaxation times in the domain (see Eq. (17)) for the calculation of the concentration field: ) ( 1 Dcat (22) 1+ τg,por = 1 and τg,cat = 2 Dpor By using variable relaxation times, the continuity of flux that is ex pected at the interface between the two media is indirectly enforced [55]. 2.3. Model assumptions To proceed to the flow and concentration field calculations, several physical assumptions were made: 1. An isothermal, Newtonian, and incompressible air flow is considered for the flow field calculations. It only takes place in the pore phase, meaning that the catalyst and substrate phases are totally imper meable to the air flow. As washcoat permeability is about ~ 10-15 m2 [45], i.e., two orders of magnitude lower than that of the cordierite substrate, this is a highly reasonable assumption. 2. The concentration of the hypothetical chemical species is assumed to be very low such that it does not impact the fluid properties. 3. The reaction of the hypothetical species occurs exclusively in the catalyst phase and is isothermal. 4. The diffusion of the hypothetical species occurs at different rates in the pore and catalyst phases. The corresponding diffusion co efficients typical for such systems are provided in Table 1. The pore space at the washcoat scale is neglected so that an effective diffusion coefficient is considered for this phase. 5. The cordierite phase is also impermeable to chemical species diffu sion and thus no reaction takes place in the cordierite.

i∕ =1

At the outlet (x = 296 × dx), a Neumann-type boundary condition was used for the concentration. This condition, commonly called outflow, forces a null diffusive flux at the outlet (i.e., D ∂∂xc = 0), which reads, at the microscopic scale, as: ∑ g2 (x, t + dt) = c(x − e2 dt, t + dt) − gi (x, t + dt) (20) i∕ =2

Lastly, at the outer domain boundaries perpendicular to the flow direction, symmetric boundary conditions were implemented, resulting in a zero mass flux going through the boundaries: − D ∂∂yc +uy c = 0 or

− D ∂∂cz +uz c = 0, where uβ is the component of the flow velocity in di rection β. In solving the ADR equation with the LBM, the symmetric boundary conditions correspond to the classical half-way bounce-back boundary condition [55], which read, respectively, as: g4 (x, t + dt) = g3 ∗ (x, t + dt) or g6 (x, t + dt) = g5 ∗ (x, t + dt)

Symbol

Additional parameters used for the simulations through all the reconstructed structures are listed in Table 1. They are based on the parameters used in [24] and are typical values for such a system [70,71]. These values lead to conversions within a transitional regime (i.e. inbetween the kinetics-limited and the mass transport-limited regimes) which is likely to occur in such systems, but care should therefore be taken not to over-generalize the conclusions of this study to all regimes. Note that the kinetics constant was varied from 1 to 106 s− 1 in an additional study to verify the impact of the rate constant on the trends obtained. Results from this additional study are also reported in Section 3. The parameters listed in Table 1 led to the following Peclet number

(21)

where * refers to the post-collision population. For the local boundary conditions, i.e., at the interface between two phases i and j inside the structure, two different treatments were needed. A half-way bounce-back boundary condition was used at the pore-cordierite and catalyst-cordierite interfaces to make the cordierite phase impermeable

7

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

Table 2 Fraction of pore volume filled by the catalyst (fw) for all reconstructed non-uniform and uniform washcoat distribution profiles averaged over the four subdomains and the corresponding standard deviation σ . Sample ID*

BW

N1

N2

N3

OS

N4

N5

N6

N7

N8

fw

0.000 0.00

0.140 0.026

0.170 0.028

0.209 0.031

0.232 0.031

0.272 0.033

0.320 0.034

0.356 0.034

0.410 0.034

0.494 0.032

σ Sample ID*

BW

U1

U2

U3

U4

fw σ (×102)

0.000 0.00

0.133 0.60

0.264 0.11

0.420 0.15

0.521 0.16

* BW: bare wall without washcoat, OS: original R&D sample, N: reconstructed non-uniform washcoat distribution profiles, U: reconstructed uniform washcoat dis tribution profiles.

for the ADR problems investigated, which implies that the stability U condition (Pex = dx Dpor ≤ 1) of the LBM scheme reported in the literature for such a problem is met (recalling that dw ≈ 24 dx) [69,72]: 0.01 ≤ Pe =

dw U ≤ 0.03≪1 Dpor

k1 dw ≤ ̃6 U k1 ≤ DaII = Lcat 2 = Φ2 ≤ ̃ 2 Dcat

̃ 2 ≤ DaI = ̃5 × 10−

(23)

3

(24)

These values show that the ADR problems investigated took place for ¨hler the most part within a transitional regime. The second Damko number (DaII ) is related to an important dimensionless number, called the Thiele modulus Φ [73], which can be used to characterize the transport limitation of the chemical species into the pore space and thus determine the effectiveness of a catalyst pellet or coating. It is shown in the literature that the catalyst effectiveness follows a specific relation ship as a function of the Thiele modulus for a given catalyst shape or coating [24,34,35,74,75]. The agreement of the simulation results with the Thiele modulus theory is verified in Section 3. Once the concentration field c(x, t) has been calculated, two impor tant catalytic performance metrics can be extracted from the results, i.e., chemical conversion X and catalyst coating effectiveness η. Because of the Dirichlet boundary condition combined with the buffer zone at the inlet of the computational domain, it is practical to define chemical conversion as:

¨hler numbers can also be calculated for characterizing the Damko prevalence of reaction through convection in the pore space (DaI ) or through diffusion in the washcoat (DaII ). They are respectively defined and bounded for the 14 structures studied in this work as:

X=

qtot,in − qtot,out qtot,in

(25)

where qtot,in and qtot,out are, respectively, the molar flux in the direc tion of the flow (x) at the inlet and the outlet of the computational domain, as defined by: qtot = − Dpor

∂c +u c ∂x x

(26)

The second metric is more specific to the washcoat context and is an indicator of how effective the catalyst coating is to the reaction. Catalyst effectiveness can be calculated through [24]:

η=

nx 1 ∑ ccat,i ni ntot i=1 cpor,i

(27)

where ccat,i and cpor,i are, respectively, the mean concentrations in the catalyst and the pore space in slice i of the computational domain (see Section 2.2.3), ntot and ni are the total number of washcoat voxels and the number of voxels in slice i, respectively, and nx = 256 is the number of slices in the x direction in the computational domain, without taking into account the added buffers. These two catalytic performance metrics of washcoat deposition were calculated for each of the 14 reconstructed structures. 3. Results and discussion Fig. 4. Evolution of the (a) surface area (S0,2,0 ) and (b) the corresponding characteristic length (Lcat ) of the catalyst phase with respect to the pore space phase, as a function of the amount of washcoat (fw ) for the two washcoat dis tribution profiles in the reconstructed GPF porous wall structures. The dashed lines are a guide for the eye, and the error bars represent the standard de viations of the reported mean values for the four wall subdomains.

The presentation of the results is divided into five parts. A charac terization of the structures using the geometrical descriptors presented in Section 2.1 is provided. The flow properties of the structures pre senting a uniform distribution compared to those with a non-uniform distribution is illustrated by flow field visualizations. The results for 8

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

Fig. 5. Visualizations of the reconstructed U2 (a) and OS (d) structures for the same 256 × 389 × 400-voxel subdomain, and their corresponding flow fields (respectively (b) and (c)) obtained from LBM simulations.

chemical conversion and catalyst coating effectiveness made it possible to assess the impact of washcoat amount and distribution uniformity on catalytic performance. The results for catalytic performance were combined with those for filtration performance reported in [25] to assess the impact of the washcoat on the overall performance of the cGPF at the microscale for two distribution profiles investigated in the present study. 3.1. Reconstructed structure characterization For every reconstructed structure, the fraction of pore volume filled fw, defined in Eq. (1), is reported as an average over the four subdomains of the whole 256 × 801 × 779-voxel structures along with its standard deviation σ, for the non-uniform and the uniform catalyst distribution series, in Table 2. The mean pore diameter (dw ) averaged over the four subdomains for each of the 14 structures investigated, as calculated using Eq. (4) from the surface area S0,1+2,0 of the solid phase (i.e., catalyst + substrate) with respect to pore space, has been reported in Fig. 6 of [25]. These results show that, for a uniform distribution profile, as every pore section is impacted by an increasing amount of washcoat, the mean pore diameter decreases gradually with an increasing fw , as intuitively expected. In the case of a non-uniform distribution profile, counterintuitively, the average mean pore diameter increases with increasing amounts of washcoat in the fw < 30% range. This result suggests that small pores are preferentially filled up as the amount of washcoat is initially increased in the case of a non-uniform coating. At higher amounts of washcoat, the mean pore diameter decreases, proving that larger pores are in turn impacted by washcoat deposition. This insight was confirmed by the pore size distribution analysis presented in [25]. These two different behaviors in the evolution of the mean pore size of the porous structure with the increase in the amount of washcoat had a significant impact on the evolution of c-GPF flow paths and catalytic performance, as presented in the following subsections. Based on the visualizations in Fig. 2, it appears that the interfacial area between the washcoat and the pore space gradually decreases as the amount of washcoat increases for reconstructed structures with a uni form washcoat distribution. On the other hand, for reconstructed structures with a non-uniform washcoat distribution, catalyst lumps appear to grow, leading to an increase in interfacial area and the clog ging of small pores as the amount of washcoat increases. This observa tion was confirmed by a surface area analysis of the two distribution

Fig. 6. Evolution of catalytic conversion (X) for a fast first-order reaction as a function of the amount of washcoat (fw ) for the two washcoat distribution profiles and all the reconstructed GPF porous wall structures. The dashed lines are a guide for the eye, and the error bars represent the standard deviations of the reported mean values for the four wall subdomains.

profiles. The surface area of the catalyst phase with respect to the pore phase (S0,2,0 ) and the corresponding characteristic length (Lcat) averaged over the four subdomains for 13 of the 14 structures investigated are reported in Fig. 4. The first observation is that S0,2,0 is significantly higher for a uniform distribution profile than for a non-uniform distribution profile for all the amounts of washcoat investigated. In the case of a uniform washcoat distribution, S0,2,0 gradually decreases as the amount of washcoat in creases due to the uniform filling of the pore volume and the resulting decrease in the interfacial area between the catalyst and the pore space. In the case of a non-uniform distribution, S0,2,0 is constrained to much lower values because of a preferential clogging of small pores as a nonuniform distribution removes a great deal of interfacial area between the washcoat and the pore space. However, as the non-uniform amount of washcoat is increased, the gradual but limited increase in surface area between the catalyst and the pores results from the significant growth of catalyst lumps, leading to an increase in the interfacial area despite further clogging of small pores, as can been seen in Fig. 2. From Fig. 4 (b), it appears that the corresponding Lcat increases gradually for the uniform washcoat distribution as the amount of washcoat is increased, 9

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

Fig. 7. Visualizations of the reconstructed U2 (a) and OS (d) structures for one 256 × 389 × 400-voxel subdomain and their corresponding concentration fields (respectively (b) and (c)) as obtained from LBM simulations considering a fast first-order reaction.

while for the non-uniform case, after an initial increase at lower amount of washcoat (fw < 30%) , Lcat reaches a more or less constant value of ~ 15 µm. These two different trends in both the evolution of S0,2,0 and thus Lcat lead to a different accessibility of the washcoat volume, which had a significant impact on the catalytic performance of the two distribution profiles, as will be presented in Sections 3.3 and 3.4.

subdomain of the OS structure), with amounts of washcoat that are as similar and typical as possible (i.e., fw ≈ 23%). It can be seen that the diameters of the flow pathways in the uniformly coated structure are globally smaller than those in the non-uniformly coated structure. This can be explained, based on the mean pore diameter results in Fig. 6 of [25] and the pore size distribution analysis in Fig. 7 of [25], by (1) the uniform narrowing of the pore paths in the case of a uniform distribution and (2) the preferential filling of the small pores leading to a redirection of the flow through the bigger pores in the case of a non-uniform dis tribution. This channeling of the flow in favor of the bigger pores in the latter case have consequences on the filtration performance of a c-GPF at the micro-scale, as highlighted in [25]. We will get back to this when the catalytic performance of the structures is analyzed.

3.2. Gas flow Once the flow field has been computed using the LBM, the flow properties of the structures, like pressure drop (ΔP) and permeability (k), can be calculated. The flow properties of the 14 structures investi gated in the present study are reported in [25]. For the sake of concision, the reader is referred to this article for a detailed description of these properties. Here, only a comparison between two flow field visualiza tions is presented in Fig. 5 to highlight some important differences be tween uniform and non-uniform structures. These visualizations show the different gas flow profiles for a uniformly coated structure (one subdomain of structure U2) and a non-uniformly coated structure (one

3.3. Catalytic conversion Once the concentration field has been computed using the LBM for each of the 14 reconstructed structures, catalytic conversion can be calculated from the data using Eq. (25). Following [24], the present study investigated a first-order reaction of a hypothetical chemical species with a kinetic rate constant k1 (see Table 1), the magnitude of which implies a fast reaction and thus a transitional regime close to a mass transport-limited regime. The conclusions set out in the following paragraphs are thus valid for this specific regime only. Nonetheless, the effect of different rate constants was also assessed. The catalytic con version values obtained for the two distribution profiles are presented in Fig. 6. As expected, catalytic conversion increases as the amount of washcoat increases for both the uniform and non-uniform distribution profiles, because more washcoat is available to the chemical species for conversion. The overall trend is similar for both distribution profiles, from a relatively sharp initial increase to a gradual flattening of the curves towards 100% conversion at high amounts of washcoat. However, the conversion for the uniform distribution series is sys tematically higher than for the non-uniform counterparts, for this firstorder reaction. A uniform distribution profile can reach up to 20% better chemical conversion than a non-uniform distribution profile in the range fw < 30%. At low amounts of washcoat, adding catalyst markedly increases the conversion of the chemical species for a uniform distribution. For a non-uniform distribution, the preferential filling of the small pores, which have a larger proportion of surface area than the larger pores, as can be deduced from Fig. 4, leads to a lower increase in chemical conversion because of the lower availability of the catalyst due to transport limitations.

Fig. 8. Evolution of the conversion (X) for a first-order reaction as a function of the rate constant (k1) for a uniform washcoat distribution profile (one sub domain of the U4 structure with fw = 52.1%) and a non-uniform distribution profile (one subdomain of the N8 structure with fw = 49.4%) in the recon structed GPF porous wall. The dashed lines are a guide for the eye. 10

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

Fig. 10. Evolution of catalyst coating effectiveness (η) for a fast first-order reaction as a function of the amount of washcoat (fw ) for the two washcoat distribution profiles in the reconstructed GPF porous wall structures. The dashed lines are to be considered at this stage as a guide for the eye (the rationale behind their actual shape will be made clearer later) and the error bars represent the standard deviations of the reported mean values for the four wall subdomains.

Fig. 9. Evolution of catalytic conversion (X) for an inhibition kinetics as a function of the amount of washcoat (fw ) for the two washcoat distribution profiles in the reconstructed GPF porous wall structures. The dashed lines are a guide for the eye, and the error bars represent the standard deviations of the reported mean values for the four wall subdomains.

It is interesting to note that the amount of washcoat needed for a uniform deposition to obtain the same conversion as the OS structure (i. e., a non-uniform distribution at fw ≈ 23%) is close to half that of the OS structure (i.e., fw ≈ 12%). Substantial catalyst reduction could thus be achieved if the uniformity of the washcoat could be improved in the case of a transitional regime close to the transport-limited regime. Fig. 7 shows the concentration fields in one subdomain of the U2 and OS structures with the fast first-order reaction. These two structures have relatively similar amounts of washcoat (i.e., fw = 26.4% and fw = 23.2%, respectively). Large differences in the concentration field pro files are observed, which can be attributed to the difference in coating uniformity. For the uniform distribution, conversion is gradual along the wall thickness whereas, for the non-uniform distribution, conversion is degraded by the presence of larger pores, which are open to the flow, devoid of catalyst, and through which most of the chemical species is transported (see Fig. 5), thus leading to lower residence times [24]. The metric that quantifies this observable result is catalyst coating effec tiveness (see Eq. (27)), the results of which are presented in the next subsection. To understand the impact of the reaction rate on the differences in conversion between uniform and non-uniform catalyst distributions, additional simulations on one subdomain of the N8 and U4 structures were conducted for different values of the rate constant k1. Considering the two structures with the highest amounts of washcoat, as done here, maximizes the differences in uniformity between the two distributions and is expected to enhance the impact on conversion. Conversion as a function of the rate constant k1 is reported in Fig. 8. The results show that the impact of the washcoat distribution profiles on conversion be comes apparent for ̃102 s− 1 ≤ k1 ≤ ̃2 × 104 s− 1, i.e., for a transition between the kinetics-limited and the transport-limited regimes, more ¨hler numbers in the range ̃0.01 ≤ DaII ≤ ̃5. precisely here for Damko At lower k1 values, conversion is low and there is virtually no difference in catalytic conversion as the catalytic regime becomes kinetics-limited. The uniformity of the catalyst coating is not an issue in this case as relatively fast diffusion makes the catalyst available no matter how uniform it is. At the other end of the spectrum, at k1 = 105 s− 1, the re action rate is so fast that only a small amount of washcoat is required and its uniformity is unimportant. Thus, generalization of the results in Fig. 6 is limited to the transport-limited regime at the one superficial velocity investigated (U = 0.055 m.s− 1). The chemical conversion results of the two washcoat uniformity distribution series indicate, as expected, that the uniform distribution is more efficient than the non-uniform distribution, but only in the

transition between the kinetics- and transport-limited regimes. Con version is also highly dependent on the amount of washcoat and the reaction rate considered. To assess the sensitivity of X to the type of reaction chosen, addi tional simulations were conducted on the two washcoat distribution series and an inhibition kinetics instead of a first-order reaction. The results are reported in Fig. 9. The first observation is that, for the kinetics constants used here, lower conversions were reached for the inhibition kinetics than for the first-order reaction studied for all washcoat amounts and levels of uni formity. The trends between the first-order reaction (Fig. 6) and the one tested with the inhibition kinetics (Fig. 9) were generally similar, i.e. an increase in conversion as the amount of washcoat is increased, but the increase is more gradual with the inhibition kinetics and the difference between a uniform and a non-uniform distribution is less important at low washcoat amount, but higher at large loadings. As a matter of fact, a mere improvement of 5% in conversion is obtained by improving the washcoat uniformity with inhibition kinetics at fw ≈ 23% (i.e. for the OS structure), whereas it is a 20% improvement for the first-order reaction. These results are obviously only valid for the kinetic constants investi gated in this work (see Table 1), i.e. for the transitional regime, as the performance should be proportional to the volume of catalyst in the kinetics-limited regime. Nonetheless, it shows that the use of a uniform washcoat distribution can also be advantageous in the case of a more complex reaction kinetics, yet the overall performance still depends on the flow and properties of the catalyst. 3.4. Catalyst coating effectiveness Chemical conversion is a good indicator of the efficiency of a specific catalytic deposition for treating harmful gases. Nonetheless, this value does not take the quantity of catalyst used to obtain such a chemical conversion performance into account. To gain a better idea of how useful the catalyst is to the conversion of the chemical species, catalyst coating effectiveness must be evaluated (see Eq. (27)). If a low con centration of chemical species is found in the catalyst, this means that only a low proportion of the catalyst contributed to the reaction, which reduces catalyst coating effectiveness. On the other hand, if a high concentration of chemical species is found in the catalyst, this means that the whole volume of catalyst contributed to the reaction, which increases catalyst coating effectiveness. Catalyst coating effectiveness (η) values for the two washcoat 11

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

space, making them harder to access by a chemical species. In the case of a non-uniform distribution, the trend is different. From the initial few catalyst nuclei that grow as more catalyst is nonuniformly added (as can be seen in Fig. 2), η rapidly drops to a value of 50%. The growth of catalyst lumps, as already discussed, results in a larger proportion of the catalyst becoming less accessible to the chem ical species and more affected by transport limitations. This phenome non takes place despite the gradual but limited growth of the interfacial area between the catalyst and the pores (see Fig. 2), which results from the expansion of the catalyst lumps. Above fw ≈ 20%, η decreases only marginally because the lower accessibility of washcoat volumes is almost counterbalanced by the growth of the interfacial area and, as a result, η levels off to a plateau at η ≈ 45%. Moreover, results in Fig. 10 show that for a fast first-order reaction, up to a 80% gain in catalyst coating effectiveness is obtained for a uniform distribution compared to a non-uniform distribution (notably at fw ≈ 23%, which corresponds to the amount of washcoat of the OS structure). This result is consistent with that of Section 3.3 showing that a 50% increase in the amount of washcoat is required to reach the same conversion when going from a uniform to a non-uniform distribution. As for chemical conversion, η was evaluated on one subdomain of the N8 and U4 structures (see Fig. 2) as a function of the kinetic constant k1. Fig. 11 shows that, in the kinetics-limited regime, for which the overall conversion is very low, as shown in Fig. 8 (i.e., for k1 ≤ ̃102 s− 1), η is similar for both washcoat distributions and is close to 100%. Beyond this threshold, i.e., from the transitional to the transport-limited regime, η decreases with the same slope for both washcoat distributions as k1 in creases. Although it was not simulated, it is expected that η would eventually go asymptotically to zero for both washcoat distributions in the case of hypothetical reaction rates k1 ≫104 s− 1, for which conversion would reach 100% (see Fig. 11), and for which only a small amount of catalyst would be required, making the thick coatings used for the U4 and N8 structures very inefficient. To further assess the validity of our numerical predictions and to compare them with the Thiele modulus theory, Fig. 12 gathers all effectiveness data presented in Figs. 10 and 11 but plotted in the usual

Fig. 11. Evolution of catalyst coating effectiveness (η) for a fast first-order reaction as a function of the rate constant (k1) for a uniform washcoat distri bution profile (one subdomain of the U4 structure with fw = 52.1%) and a nonuniform distribution profile (one subdomain of the N8 structure with fw = 49.4%) in the reconstructed GPF porous wall. The dashed lines are a guide for the eye.

1/2

log–log plot as a function of the generalized Thiele modulus Φ = DaII (see Eq. (24)). The effectiveness data for all the reconstructed structures nearly collapse into a single curve which suggests the possible existence of a universal correlation describing all effectiveness data. In a log–log plot of η as a function of Φ, one would expect the η curves for all reconstructed structure series to converge at high Φ towards a η = 1 Φ asymptotic line, as already shown with other catalysts of various shapes by [73]. To illustrate this expected behavior, the effectiveness curves from the textbook examples of a flat catalyst slab and a spherical catalyst are also included in Fig. 12. However, as can be seen in Fig. 12, the computed effectiveness of the reconstructed washcoats do not converge towards the expected limit. Rather, the data converge towards a line shifted to the left of the graph, i.e. η = α1Φ, where α is a parameter greater than one describing the shift of the asymptote. Here, the data of uniform and non-uniform distribution profiles are well described by an α value of about 1.4. For the discussion of the origin of the unexpected shift in the asymptote, it is useful to recall that the computed Thiele modulus is here defined in terms of a characteristic length that is calculated as the ratio of the volume of the catalyst phase divided by the pore-catalyst inter facial area (see Eq. (3)). While the catalyst volume is well defined, the determination of the interfacial area is more ambiguous. The need to apply the additional correction parameter α of about 1.4 suggests that the used procedure overestimates the effective interfacial area by more than the geometrical correction factor of 1.5 already applied here, as mentioned earlier, to account for the voxelized surface as suggested by [58,59]. The most likely explanation for this overestimation of the effective interfacial area is that the structure data includes information of a microstructure that is below the characteristic length of the reaction

Fig. 12. Evolution of catalyst coating effectiveness (η) for a first-order reaction as a function of the Thiele modulus (Φ) for uniform (red symbols) and nonuniform (green symbols) washcoat distribution profiles in the reconstructed GPF porous wall (combined data from both Figs. 10 and 11), fitted through weighted non-linear regressions with Eq. (28) (red and green dashed curves respectively) and compared with relationships from the Thiele modulus theory for slab-shaped and spherical catalyst pellets [76,77]. The black line represents the theoretical 1/Φ relationship expected at high Thiele moduli. (For inter pretation of the references to colour in this figure legend, the reader is referred to the web version of this article.)

distribution profiles are shown in Fig. 10 for a fast first-order reaction, i. e., conditions corresponding to the transitional regime close to the transport-limited regime. Fig. 10 shows that η decreases in tandem with an increase in the amount of washcoat for both distributions. This first observation is very intuitive, given that a greater proportion of the washcoat volume is less easily accessible by the chemical species as the amount of catalyst is increased. In the case of a uniform distribution, η decreases more gradually from the 100% effectiveness obtained with a very thin catalyst coating. This is due to the homogeneous incre mentation of the thickness of the catalyst, which gradually increases the catalyst volume while the interfacial area between the washcoat and the pore space decreases (as can be seen in Fig. 4). This drives additional catalyst volumes further and further from the interface with the pore 12

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

Table 3 Fitted parameters for Eq. (28) and quality of the non-linear regressions for the uniform and non-uniform washcoat distribution data as well as the aggregated data. Parameter

Uniform washcoat distributions

Non-uniform washcoat distributions

All washcoat distributions

n(-)

1.43 ± 0.05

1.27 ± 0.11

1.54 ± 0.06

α(-)

1.48 ± 0.13

1.44 ± 0.17

1.87 ± 0.13

2.95 × 10-6

2.15 × 10-6

3.70 × 10-12

0.997

0.991

0.995

p-value (n) p-value (α) R2

7.93 × 10-8

4.78 × 10-8

7.14 × 10-17

diffusion problem. Such microstructure below the characteristic diffu sion length has little impact on the computed concentration profiles and thus on the computed effectiveness, whereas it increases the nominal interfacial area and consequently leads to an underestimation of the Thiele modulus. The observed shift in the high-Thiele modulus asymptote is consis tent with the earlier results reported in [24] where the effect of intrapore diffusion limitations on the effectiveness of catalytically coated filters were described. In that work, the characteristic length was used as a fitting parameter in order to represent the pore scale simulation results for the catalyst coating effectiveness. In order to fit the pore-scale sim ulations, the characteristic length obtained based on the voxelized interfacial area had to be increased by a factor of 2.1. In the current work, the combined correction by the geometrical correction factor of 1.5 and the shift parameter α of ~ 1.4 results in an identical total correction by a factor of 2.1. Besides the difficulties in determining the effective interfacial area from the micro-structured geometry, mass transport limitations in the open pores might also contribute to the observed shift in high-Thielemodulus asymptote. The simulations show some concentration gradi ents also in the gas phase and this suggests that diffusion in the open gas phase might contribute to the observed loss in catalyst coating effec tiveness. Such external mass transfer limitations are neglected in the current analysis. Furthermore, future work needs to investigate the ef fect of the resolution of the tomography on the computed catalyst coating effectiveness. It is common practice to perform pore scale sim ulations directly from the voxelization obtained from the reconstruction of the tomographic data. For high reaction rates (high Thiele moduli), the resolution of the tomographic images might be insufficient to cap ture the strong gradients occurring at the catalyst interface and thus might lead to a numerical overestimation of diffusion limitations. While it seems unsatisfactory to apply the correction factor α and further work is needed to elucidate the exact cause of the observed de viations from the 1/Φ asymptote, from a practical standpoint, the observation that the coating effectiveness for the different catalyst dis tributions can be represented by a single master curve is of substantial value, since it allows a convenient implementation of the observed pore scale diffusion limitations into reactor scale models. To this end, the common two-parameter correlation proposed by [75,78] is here rear ranged to account for the parameter α earlier defined such that: (

η=

1 1 + αΦn

)1/n

Fig. 13. Example of the quantification of possible improvements in filtration (a) and catalytic (b) performance by changing from a non-uniform to a uniform washcoat distribution for the N3 structure (fw = 20.9%) as predicted by the results presented both in the present study (b) and in [25] (a).

data fitted to Eq. (28), n is found to vary within a relatively limited range (i.e. 1.27 ≤ n ≤ 1.43) for the two washcoat distributions studied and α can be considered as being more or less constant at around 1.46. Despite the very different washcoat distributions, the data for the uniform and non-uniform washcoats are both well described by an aggregate corre lation with n = 1.54 and α = 1.87 (not plotted in Fig. 12). This suggests that this correlation provides a good starting point for the description of diffusion limitation in arbitrary coated particulate filters. As a verifica tion of the ability of the aggregate correlation to describe catalyst effectiveness as a function of washcoat amount for different catalyst distributions, the guides for the eye of Fig. 10 were actually calculated using the aggregate correlation proposed here and the characteristic length data of Fig. 4. As can be seen, the aggregate correlation pre dictions offer a very good fit of the data for the two distribution profiles with average and maximum relative deviations of 1.3% and 4.1% respectively. Given the wide range of catalyst structure investigated, this result suggests that the proposed correlation provides a good description for general washcoat distributions. Despite the effort to provide a single correlation, one can still note in Fig. 12 that the Thiele modulus threshold at which the decay of the catalyst coating effectiveness takes place, i.e. when mass transport limitation starts to become dominant, slightly varies for the different coating uniformities, in a way similar to a change of catalyst shape, i.e. going from sphere (blue dashed curve in Fig. 12) to slab (orange dashed curve in Fig. 12). As a matter of fact, washcoats with a more rounded or spherical shape, i.e. non-uniform coatings (see Fig. 2), yield for a given Φ slightly lower η values than uniform coatings that can be regarded as a

(28)

where n is a fitted parameter that is expected to depend on the “shape” of the washcoat deposition. The two parameters n and α were here fitted through weighted nonlinear regressions, giving four times as much weight to the mean values (data from Fig. 10) as to the data point of a single subdomain (data from Fig. 11). In a first step, separate fits were performed for the two data sets with uniform and non-uniform washcoat distributions. As can be seen in Table 3 reporting the regression parameters obtained for the numerical 13

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

quality factor (Qf), which is an intrinsic filter property independent of ) ( filter thickness and is defined as Qf = − ln 1 − Ef /ΔP, with Ef being soot capture efficiency at the most penetrating particle size and ΔP being pressure drop through the filter. Although the better overall perfor mance (i.e. both in terms of filtration and catalytic conversion) of a uniform distribution compared to a non-uniform distribution may seem to be an expected result for chemical reaction engineers, the numerical models developed here and in a previous study [25] are capable of quantifying precisely the difference in overall CPF performance. It can thus provide engineers with guidelines for determining the best strategy to improve performance, such as working on better uniformity and/or increasing the amount of washcoat. To illustrate this, Fig. 13 provides a comparison of both the filter quality factor (reported in Fig. 16 from [25]) and catalytic conversion between the uniform and non-uniform washcoat distributions investigated in the present study. For example, one can see that the quality factor improves by 50% (corresponding to a ̃10% relative decrease in ΔP and relative capture efficiency improve ment by ̃70%, as shown in Figs. 9 and 11, respectively, in [25]) and the catalytic conversion by 20% by improving the uniformity of the catalyst coating distribution of the N3 sample (fw = 20.9%). Such precise quantifications of possible improvements obtained by refining washcoat uniformity represents valuable information for researchers interested in optimizing the overall performance of a CPF.

Fig. 14. Schematic of the cuboidal domain and operating conditions employed for the pseudo-3D advection–diffusion test case used to verify the LBM code implemented for the present study. The red dashed line represents the direction along which the concentration data were gathered. (For interpretation of the references to colour in this figure legend, the reader is referred to the web version of this article.)

4. Conclusion Following a previous work by [25], which studied the impact of washcoat amount and uniformity on the filtration performance of a catalyst-coated gasoline particulate filter (c-GPF) at the wall scale, a three-step numerical model is proposed here to predict the catalytic performance of a c-GPF. It consists of (1) reconstructing representative elementary volumes of the porous walls of the c-GPF using tomographic images processed by a set of morphological image operations, and of (2) computing the flow field and (3) the concentration field following a fast first-order reaction of a hypothetical chemical species within the c-GPF wall using in-house LBM solvers. This approach can be used to predict and compare the catalytic conversion and catalyst coating effectiveness of a c-GPF wall with a uniform or a non-uniform washcoat distribution and different washcoat amounts. Although other forms of washcoat deposition exist, such as on-wall depositions, which have been numer ically studied in [44-48,80] and shown to affect the CPF performance, the current study focuses on in-wall washcoat depositions. Although caution should be exercised when generalizing the findings reported here to all non-uniform in-wall washcoat depositions, all c-GPF wall substrates and all operating conditions, the following conclusions can be drawn from the present study:

Fig. 15. Concentration profile at steady state along the red dashed line of Fig. 14 for different grid spacings using the LBM compared to the analytical solution found in [85] and the solution obtained using COMSOL Multiphysics® software. (For interpretation of the references to colour in this figure legend, the reader is referred to the web version of this article.)

collection of slabs. A similar deviation is indeed observed between the spherical catalyst pellets and slab-shaped catalyst layers. Overall, these results are important as they provide a tool for catalyst design and guidance for the optimization of the catalyst deposition process. They are also relevant for the simulation community, since they show that a quantitative description of the reactive flow in the wall can be achieved by means of a homogeneous wall model without the need of further detailed pore scale simulations. Provided that the microstructure below the characteristic length relevant to the reaction–diffusion prob lem can be filtered out, the required catalyst washcoat effectiveness could be determined directly from the washcoat geometry (e.g. by X-ray computed tomography, as has been done here, or possibly by mercury intrusion porosimetry [79]) without the need for pore-scale simulations or conversion measurements. Further research is however required to characterize more precisely the relevant surface structures.

• For the cordierite substrate investigated, catalytic conversion in creases markedly for both the uniform and non-uniform washcoat distributions with up to 30% of the pore volume filled with washcoat. However, the uniform coating provides up to ~ 20% better conver sion for a fast first-order reaction. Beyond these amounts of wash coat, only a marginal improvement can be obtained. • The difference in catalytic conversion between the two types of washcoat uniformity is mainly apparent within the transitional regime, that is, between the kinetics- and transport-limited regimes, ¨hler numbers in the range ̃0.01 ≤ DaII ≤ ̃5. This differ for Damko ence can be explained by the lower specific surface area between the catalyst and the pores for the non-uniform distribution, which results from the clogging of the small pores, making a large fraction of catalyst unavailable for reaction. • Catalyst coating effectiveness for a fast first-order reaction gradually decreases as the amount of washcoat is increased for a uniform deposition, whereas catalyst coating effectiveness drops sharply for a non-uniform deposition with a low amount of washcoat. The latter

3.5. Overall performance As reported in the present work, structures with a uniform washcoat distribution displayed a better catalytic performance than structures with a non-uniform washcoat distribution investigated here. In a pre vious study [25], it was also shown that uniformly coated structures perform better in terms of filtration performance as measured by a filter 14

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

Fig. 16. Schematic of the concentric square material test case. The red dashed line represents the direction along which the concentration data were gathered for the comparison. (For interpretation of the references to colour in this figure legend, the reader is referred to the web version of this article.)

Fig. 19. Concentration profile along the red dashed line of Fig. 18 for different values of the kinetic and inhibition constants k1 (in s− 1) and K (in m3/mol) with the LBM code compared to the solutions obtained with COMSOL Multiphysics® software. (For interpretation of the references to colour in this figure legend, the reader is referred to the web version of this article.) Table 4 Comparison of conversion and catalyst efficiency in the OS structure as calcu lated with the LBM and GeoDict®. X

η

LBM (current work)

PoreChem/GeoDict® Greiner et al. (2019)

0.743 0.495

0.749 0.477

within the structure. The apparent shift is largely attributed to an overestimation of the effective interfacial area, and thus to an un derestimation of the washcoat characteristic length, which most probably results from taking into account, in the interfacial area calculation, surface microstructures that are not per se relevant to the diffusion–reaction problem.

Fig. 17. Concentration profile along the red dashed line of Fig. 16 for different values of the kinetics constant k1 (in s− 1) using the LBM code compared to the solutions obtained using COMSOL Multiphysics® software. (For interpretation of the references to colour in this figure legend, the reader is referred to the web version of this article.)

Using results from [25], a case study demonstrated how the proposed numerical model can be a valuable and quantitative approach that can provide insights into whether and why specific catalyst coatings perform better than others in terms of filtration and catalytic performance, and thus provide guidance for particulate filter researchers and manufac turers for improving exhaust gas aftertreatment devices. This case study showed that a uniform washcoat distribution outperforms the nonuniform washcoat distribution studied in terms of both filtration and catalytic functionalities. Although this result could have been antici pated, the proposed model makes it possible to quantify the improve ments that can be expected. Lastly, it is interesting to note that, as the LBM approach used here is an intrinsically transient and highly parallelizable computational method, the authors believe that the proposed approach would be wellsuited to study the time evolution of many concurrent reactions under varying conditions, such as for studying the impact of catalyst oxygen storage on NOx, CO, and HC emissions. This would require solving as many ADR problems as there are species involved in these reactions and deploying the resulting coupled computations on a highperformance GPU cluster, a solution that is capable of substantially accelerating the computations [81,82]. This will be the subject of a future study.

Fig. 18. Schematic of the inhibition kinetics reaction test case. The red dashed line represents the direction along which the concentration data were gathered for the comparison. (For interpretation of the references to colour in this figure legend, the reader is referred to the web version of this article.)

trend can be explained by the nature of the non-uniformity studied, which consists of catalyst lumps expanding in size as the amount of washcoat is increased and which makes initially deposited volumes of washcoat less and less accessible because of chemical species transport limitations. Up to an 80% gain in catalyst coating effec tiveness for a uniform distribution can be obtained compared to a non-uniform distribution for this reaction. • The computed catalyst coating effectiveness data can be fitted to a two-parameter correlation that is broadly consistent with the Thiele modulus theory, with the notable exception of an apparent shift to lower Thiele moduli. This correlation underlines the importance of both the characteristic length, defined as the ratio of the volume of the catalyst phase to an effective interfacial surface of the catalyst, and of parameter n that is related to the overall shape of the catalyst

Declaration of Competing Interest The authors declare that they have no known competing financial 15

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

Fig. 20. Comparison of the concentration field of a 2D slice obtained through the OS structure as computed using the LBM implementation (left) and PoreChem/ GeoDict® (right).

interests or personal relationships that could have appeared to influence the work reported in this paper.

(STPGP-493797-16) and a Grant from the Collaborative Research and Training Experience (CREATE-481695-2016) program in Simulationbased Engineering Science (G´ enie Par la Simulation). The authors would also like to thank Calcul Qu´ebec/Compute Canada for the computational resources and support provided. Work at TU Darmstadt was funded by Bundesministerium für Bildung und Forschung in the framework of the project ML-MORE (05M20RDA).

Acknowledgements This research was supported by the Natural Sciences and Engineering Research Council of Canada through a Strategic Partnership Grant

Appendix A. – LBM CODE VERIFICATION, ACCURACY ASSESSMENT AND COMPUTATIONAL PERFORMANCE In this section, several verifications of the LBM code implemented to solve the ADR equation is carried out by comparing the results obtained with those from an analytical solution and/or from commercial COMSOL Multiphysics® software, for relatively simple test cases. A comparison with the concentration field in the OS structure obtained with GeoDict® software [83], as reported in [24], is then provided to assess the accuracy of the implementation for a complex porous structure. Note that an exhaustive validation of the LBM code implemented for flow simulations in the reconstructed porous wall structures can be found in [84]. Lastly, the computational performance of the code is reviewed. A.1 Code verification To verify the calculation of the concentration field of a hypothetical chemical species using the LBM code implemented for the present study, three test cases were performed. A.1.1 First-order reaction in a two-phase medium The first verification test case illustrated in Fig. 14 consisted of a hypothetical pseudo-3D advection–diffusion problem of a species in a cuboidal domain split into two equal parts having a ratio of diffusion coefficients of the species into their respective medium of D2/D1 = 20. The transport velocity of the species was uniform throughout the domain, pointing in the x-direction and set to U = L/t1 m/s, where L is the length of the rectangular domain in the direction of the flow and t1 is a time period of 1 s. Furthermore, the diffusion coefficient in Medium 1 was defined such that D1 = L2/t2 with t2 = t1/20. The outer domain boundary conditions were set to be symmetric in the directions perpendicular to the flow (y,z). Two Dirichlet boundary conditions were used at the inlet (c = 0 mol/l) and outlet (c = c0 = 1 mol/l) of the domain. The results presented in Fig. 15 and obtained with the LBM for different grid spacings (dx) were compared to an analytical solution reported in [85] as well as to the solution obtained using commercial COMSOL Multiphysics® software (version 5.2a) at the finest mesh possible. Very good agreement between all the approaches used to solve this verification test case was found. The mean relative discrepancies for the three LBM grid resolutions with respect to the analytical solution were 3.5%, 1.6% and 0.7%, respectively. Only a slight discrepancy is apparent in the quadratic sharp variation region just before the transition between the 2D media, for which sufficient LBM grid spacing was required to achieve an accurate solution. This gives confidence in the accuracy of the advection–diffusion LBM solver implemented in the present study. An L2-error firstorder convergence was obtained for the LBM implementation, which is consistent with the results reported in [55] for this LBM implementation in the case of an ADR equation. A.1.2 First-order reaction in a concentric two-phase medium This verification test case consists of a channel with a square section presenting two hypothetical media labeled 1 and 2, as shown in Fig. 16. The ratio between the two diffusion coefficients is D1/D2 = 65, and the velocity is uniform in Medium 1 and set to U = L/t1 m/s, with t1 = 1 s, D1 = L2/t2, and t2 = t1/20. A first-order reaction takes place exclusively in Medium 2. Dirichlet boundary conditions are set at the inlet (c = 0 mol/l in Medium 2 and c = c0 = 1 mol/l in Medium 1) and an outflow boundary condition at the outlet (i.e., D ∂∂xc = 0). The results were compared to those obtained using commercial COMSOL Multiphysics® software. Fig. 17 shows that there is very good agreement between the results of the two programs. 16

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040

A.1.3 Inhibition kinetics reaction in a single-phase medium This test case consists of a square channel of one phase as shown in Fig. 18 where the inhibition kinetics reaction takes place. The velocity is uniform and is set to U = L/t1 m/s, with t1 = 1 s. A Dirichlet boundary condition is set at the inlet (c = c0 = 1 mol/l) and an outflow boundary condition at the outlet (i.e., D ∂∂xc = 0). The diffusion coefficient is set to D1 = L2/t2 with t2 = t1/20. The results were compared to those obtained with commercial COMSOL Multiphysics® software. As can been seen in Fig. 19, very good agreement was found for the different kinetics parameters of k1 and K. A.2 Accuracy assessment To evaluate the coupled LBM implementation in the context of an ADR problem for a first-order reaction through a complex porous structure, the 256 × 801 × 779-voxel OS structure shown in Fig. 3 in [25], the concentration field of a hypothetical chemical species was computed and was compared with results reported in [24] and obtained using the finite volume PoreChem simulation tool combined with the GeoDict® SimpleFFT flow solver. The physical parameters used for these simulations are those reported in Table 1. The grid spacing (dx) used here for the comparison was 1.4 µm. The performance metrics are compared in Table 4. A relative difference of 0.8% for X and 3.8% for η were obtained. This small discrepancy can be attributed to the difference in buffer size used upstream and downstream from the structure (20 voxels in the present simulation vs. 100 voxels in [24]). A visualization of the two concentration fields in the top section of the computational domain (y = 779 × dx) is also provided in Fig. 20. Two similar profiles were obtained, which gives confidence in the concentration field computations implemented in the present study. A.3 Computational performance The overall computational time for the LBM flow calculations on a 456 × 400 × 389-voxel porous wall subdomain was approximately 6 h on 8 cores of a 2.67 GHz Intel Xeon X5650 Westmere processor computer. The simulations used approximately 3.5 GB of RAM. For the concentration field calculations on a 296 × 400 × 389-voxel porous wall subdomain, the computational time was approximately 30 h on 12 cores of a 2.67 GHz Intel Xeon X5650 Westmere processor computer. The relative long computational time for the transient solution of the concentration field could be reduced by further code optimization. The simulations used approximately 15 GB of RAM.

References [21]

[1] World Health Organization, Ambient air pollution, A global assessment of exposure and burden of disease, Switzerland, Geneva, 2016. [2] K. Zhang, S. Batterman, Air pollution and health risks due to vehicle traffic, Sci. Total Environ. 450-451 (2013) 307–316. [3] B. Guan, R. Zhan, H.e. Lin, Z. Huang, Review of the state-of-the-art of exhaust particulate filter technology in internal combustion engines, J. Environ. Manage. 154 (2015) 225–258. [4] C. Ozhan, D. Fuster, P. Da Costa, Multi-scale flow simulation of automotive catalytic converters, Chem. Eng. Sci. 116 (2014) 161–171. [5] J.M. Richter, R. Klingmann, S. Spiess, K.-F. Wong, Application of Catalyzed Gasoline Particulate Filters to GDI Vehicules SAE International Journal of Engines 5 (2012) 3. [6] A. Ricca, V. Palma, M. Martino, E. Meloni, Innovative catalyst design for methane steam reforming intensification, Fuel 198 (2017) 175–182. [7] B.A.A.L. van Setten, M. Makkee, J.A. Moulijn, Science and technology of catalytic diesel particulate filters, Catalysis Reviews 43 (4) (2001) 489–564. [8] S. Lorentzou, C. Pagkoura, A.G. Konstandopoulos, J. Boettcher, Advanced Catalyst Coatings for Diesel Particulate Filters, SAE Int. J. Engines 01 (0483) (2008). [9] J. Wang, H. Chen, Z. Hu, M. Yao, Y. Li, A Review on the Pd-Based Three-Way Catalyst, Catalysis Reviews 57 (1) (2015) 79–144. [10] S.F. Benjamin, Z. Liu, C.A. Roberts, Automotive catalyst design for uniform conversion efficiency, Appl. Math. Model. 28 (6) (2004) 559–572. [11] S. Lorentzou, C. Pagkoura, A. Zygogianni, G. Kastrinaki, A.G. Konstandopoulos, Catalytic Nano-structured Materials for Next Generation Diesel Particulate Filters, SAE Int. J. Mater. Manf. 1 (1) (2009) 189–198. [12] J. Czerwinski, Y. Zimmerli, A. Mayer, G. D’Urbano, D. Zürcher, Emission Reduction with Diesel Particle Filter with SCR Coating (SDPF), Emiss. Control Sci. Technol. 1 (2) (2015) 152–166. [13] M. V´ aclavík, M. Plach´ a, P. Koˇcí, M. Svoboda, T. Hotchkiss, V. Nov´ ak, D. Thompsett, Structure characterisation of catalytic particulate filters for automotive exhaust gas aftertreatment, Mater. Charact. 134 (2017) 311–318. [14] V. Palmaa, P. Ciambellia, E. Melonia, A. Sinb, Optimal CuFe2O4 Load for MW Susceptible Catalysed DPF, Chem. Eng. Trans. 35 (2013) 727–732. [15] K.G. Rapp´e, Integrated Selective Catalytic Reduction–Diesel Particulate Filter Aftertreatment: Insights into Pressure Drop, NO x Conversion, and Passive Soot Oxidation Behavior, Ind. Eng. Chem. Res. 53 (45) (2014) 17547–17557. [16] C.K. Lambert, M. Bumbaroska, D. Dobson, J. Hangas, J. Pakko, P. Tennison, Analysis of High Mileage Gasoline Exhaust Particle Filters, SAE Int. J. Engines 9 (2) (2016) 1296–1304. [17] A. Fiano, A model for soot load estimation in a Gasoline Particulate Filter using a Radio Frequency sensor, University of Windsor, 2017. [18] C. Lambert, T. Chanko, D. Dobson, X. Liu, J. Pakko, Gasoline Particle Filter Development, Emiss. Control Sci. Technol. 3 (1) (2017) 105–111. [19] A. Joshi, T.V. Johnson, Gasoline Particulate Filters—a Review, Emiss. Control Sci. Technol. 4 (4) (2018) 219–239. [20] D. Lopez-Gonzalez, M.N. Tsampas, A. Bor´eave, L. Retailleau-Mevel, M. Klotz, C. Tardivat, B. Cartoixa, K. Pajot, P. Vernoux, Mixed Ionic–Electronic Conducting

[22] [23] [24]

[25] [26] [27] [28]

[29] [30]

[31] [32] [33] [34] [35] [36] [37]

17

Catalysts for Catalysed Gasoline Particulate Filters, Top Catal 58 (18-20) (2015) 1242–1255. S. Inoda, Y. Nomura, H. Ori, Y. Yabuzaki, Development of New Coating Technology Optimized for Each Function of Coated GPF, SAE Technical Paper Series. (2017). K. Tsuneyoshi, O. Takagi, K. Yamamoto, Effects of Washcoat on Initial PM Filtration Efficiency and Pressure Drop in SiC DPF, SAE Technical Paper. 01 (0817) (2011) 10. M.A. Mitsouridis, D. Karamitros, G. Koltsakis, Model-Based Analysis of TWCCoated Filters Performance, Emiss. Control Sci. Technol. 5 (3) (2019) 238–252. R. Greiner, T. Prill, O. Iliev, B.A.A.L. van Setten, M. Votsmeier, Tomography based simulation of reactive flow at the micro-scale: Particulate filters with wall integrated catalyst, Chem. Eng. J. 378 (2019) 121919, https://doi.org/10.1016/j. cej.2019.121919. I. Belot, D. Vidal, M. Votsmeier, R. Hayes, F. Bertrand, Numerical Investigation of the Impact of Washcoat Distribution on the Filtration Performace of Gasoline Particulate Filters, Chem. Eng. Sci. 221 (115656) (2020). A.G. Konstandopoulos, M. Kostoglou, N. Vlachos, The multiscale nature of diesel particulate filter simulation, IJVD 41 (1/2/3/4) (2006) 256, https://doi.org/ 10.1504/IJVD.2006.009676. Koltsakis G, Haralampous O, Depcik C, Ragone JC. Catalyzed diesel particulate filter modeling. Reviews in Chemical Engineering. 2013;29(1):1-61. Y. You, Z. Wu, W. Zeng, Z. Zhang, S. Wang, F. Dai, Z. Yi, CFD modeling of unsteady SCR deNOx coupled with regenerative heat transfer in honeycomb regenerators partly coated by Vanadium catalysts, Chem. Eng. Res. Des. 150 (2019) 234–245. S. Hajireza, L. Johannesen, T. Wolff, G. Koltsakis, Z. Samaras, O. Haralampous, A modeling and experimental investigation on an innovative substrate for DPF applications, SAE Int. J. Engines 01 (0891) (2010). K.C. Premchand, Development of a 1-D Catalyzed Diesel Particulate Filter Model for Simulation of the Performance and the Oxidation of Particulate Matter and Nitrogen Oxides Using Passive Oxidation and Active Regeneration Engine Experimental Data, Michigan Technological University (2013). S.F. Benjamin, C.A. Roberts, Methodology for Modelling a Combined DPF and SCR Catalyst with the Porous Medium Approach in CFD, SAE Int. J. Engines 7 (4) (2014) 1997–2011. J.C. Wurzenberger, S. Bardubitzki, S. Kutschi, R. Fairbrother, C. Poetsch, Modeling of Catalyzed Particulate Filters - Concept Phase Simulation and Real-Time Plant Modeling on HiL, SAE Int. J. Engines 9 (3) (2016) 1720–1734. S. Olowojebutu, T. Steffen, A Review of the Literature on Modelling of Integrated SCR-in-DPF Systems, SAE Technical Paper Series. (2017). R.E. Hayes, B. Liu, M. Votsmeier, Calculating effectiveness factors in non-uniform washcoat shapes, Chem. Eng. Sci. 60 (7) (2005) 2037–2050. R.E. Hayes, P.K. Mok, J. Mmbaga, M. Votsmeier, A fast approximation method for computing effectiveness factors with non-linear kinetics, Chem. Eng. Sci. 62 (8) (2007) 2209–2215. D. Karamitros, G. Koltsakis, Model-based optimization of catalyst zoning on SCRcoated particulate filters, Chem. Eng. Sci. 173 (2017) 514–524. J. Lee, J.R. Theis, E.A. Kyriakidou, Vehicle emissions trapping materials: Successes, challenges, and the path forward, Appl. Catal. B 243 (2019) 397–414.

I. Belot et al.

Chemical Engineering Journal 406 (2021) 127040 [62] D. Vidal, R. Roy, F. Bertrand, A parallel workload balanced and memory efficient lattice-Boltzmann algorithm with single unit BGK relaxation time for laminar Newtonian flows, Comput. Fluids 39 (8) (2010) 1411–1423. [63] T. Toffoli, N.H. Margolus, Invertible cellular automata: A review, Physica D 45 (13) (1990) 229–253. [64] Z. Guo, C. Shu, Lattice Boltzmann Method and Its Applications in Engineering, World Scientific, Singapore, 2013. [65] P.L. Bhatnagar, E.P. Gross, M. Krook, A Model for Collision Processes in Gases. I. Small Amplitude Processes in Charged and Neutral One-Component Systems, Phys. Rev. 94 (3) (1954) 511–525. [66] F. Bertrand, C. Devals, D. Vidal, C. S´ eguineau de Pr´eval, R.E. Hayes, Towards the simulation of the catalytic monolith converter using discrete channel-scale models, Catal. Today 188 (1) (2012) 80–86. [67] R.B. Bird, W.E. Stewart, E.N. Lightfoot. Transport Phenomena, Edition, John Wiley & Sons, Inc, 2007. [68] S.E. Vollz, C.R. Morgan, D. Liederman, S.M. Jacob, Kinetic Study of Carbon Monoxide and Propylene Oxidation on Platinum Catalysts, Ind Eng Chem, Prod Res Develop. 12 (4) (1973) 8. [69] S.A. Hosseini, N. Darabiha, D. Th´ evenin, A. Eshghinejadfard, Stability limits of the single relaxation-time advection–diffusion lattice Boltzmann scheme, Int. J. Mod. Phys. C 28 (12) (2017) 1750141, https://doi.org/10.1142/S0129183117501418. [70] F. Zhang, R.E. Hayes, S.T. Kolaczkowski, A New Technique to Measure the Effective Diffusivity in a Catalytic Monolith Washcoat, Chem. Eng. Res. Des. 82 (4) (2004) 481–489. [71] E.N. Fuller, P.D. Schettler, J.C. Giddings, New method for prediction of binary gasphase diffusion coefficients, Ind. Eng. Chem. 58 (5) (1966) 18–27. [72] S. Suga, Stability and accuracy of the lattice Botlzmann schemes for anisotropic advection-diffusion equations, Int. J. Mod. Phys. C 20 (04) (2009) 633–650. [73] R. Aris, On shape factors for irregular particles—I, Chem. Eng. Sci. 6 (6) (1957) 262–268. [74] O. Deutschmann, Modeling of the Interactions Between Catalytic Surfaces and GasPhase, Catal Lett 145 (1) (2015) 272–289. [75] R.E. Hayes, J.P. Mmbaga, Chapter 9: Transport Processes In Catalysis, in: H. C. Press (Ed.), Introduction to Chemical Reactor Analysis, Second Edition, 2012. [76] S. Liu, Bioprocess Engineering : Kinetics, Sustainability, and Reactor Design, 2 ed:, Elsevier, 2017, p. 1172 p.. [77] P.M. Doran, Bioprocess Engineering Principles, 2 ed:, Academic Press, 2013, p. 926 p.. [78] D. Leung, R.E. Hayes, S.T. Kolaczkowski, Diffusion limitation effects in the washcoat of a catalytic monolith reactor, Can. J. Chem. Eng. 74 (1) (1996) 94–103. [79] X.Q. Yan, C.Y. Zhou, Y.G. Fang, L.S. Lin, Experiment Study on Determination of Surface Area of Finegrained Soils by Mercury Intrusion Porosimetry, IOP Conf. Ser.: Earth Environ. Sci. 100 (2017) 012003, https://doi.org/10.1088/1755-1315/ 100/1/012003. [80] P. Koˇcí, Multi-scale modeling of catalytic particulate filtes for gasoline engines (GPF). International Symposium on Modeling of Exhaust-Gas After-Treatment (MODEGAT, Bad Herrenalb/Karlsruhe, Germany, 2019. [81] Leclaire S, Vidal D, Fradette L, Bertrand F, editors. Lattice Boltzmann Modeling of Immiscible Liquid-Liquid Flows in Static Mixers. Mixing XXVI; 2018; San Juan, Porto Rico, USA. [82] E. Calore, A. Gabbana, J. Kraus, E. Pellegrini, S.F. Schifano, R. Tripiccione, Massively parallel lattice–Boltzmann codes on large GPU clusters, Parallel Comput. 58 (2016) 1–24. [83] 2018 ed., Math2Market GmbH, www.geodict.com, 2018. [84] I. Belot, Y. Sun, D. Vidal, M. Votsmeier, P. Causse, F. Trochu, F. Bertrand, A 3D additive manufacturing approach for the validation of a numerical wall-scale model of catalytic particulate filters, Chem. Eng. J. 405 (2021) 126653, https:// doi.org/10.1016/j.cej.2020.126653. [85] H. Karani, C. Huber, Lattice Boltzmann formulation for conjugate heat transfer in heterogeneous media, Phys. Rev. E 91 (2) (2015), https://doi.org/10.1103/ PhysRevE.91.023304.

[38] A.G. Konstandopoulos, M. Kostoglou, S. Lorentzou, N. Vlachos, Aspects of multifunctional diesel particulate filters and their efficient simulation, Catal. Today 188 (1) (2012) 2–13. [39] H. Hayashi, S. Kubo, Computer simulation study on filtration of soot particles in diesel particulate filter, Comput. Math. Appl. 55 (7) (2008) 1450–1460. [40] D.Y. Lee, G.W. Lee, K. Yoon, B. Chun, H.W. Jung, Lattice Boltzmann simulations for wall-flow dynamics in porous ceramic diesel particulate filters, Appl. Surf. Sci. 429 (2018) 72–80. [41] G. Matte-Deschˆenes, D. Vidal, F. Bertrand, R.E. Hayes, Numerical investigation of the impact of thermophoresis on the capture efficiency of diesel particulate filters, Can. J. Chem. Eng. 94 (2) (2016) 291–303. [42] M. Stewart, T. Gallant, D. Kim, G. Maupin, A. Zelenyuk, Fuel Efficient Diesel Particulate Filter (DPF) Modeling and Development. Pacific Northwest National, Laboratory. (2010). [43] S. Tsushima, I. Nakamura, S. Sakashita, S. Hirai, D. Kitayama, Lattice Boltzmann Simulation on Particle Transport and Captured Behaviors in a 3D-Reconstructed Micro Porous DPF. SAE, International. (2010). ˇ ep´ [44] P. Koˇcí, F. Stˇ anek, M. Kubíˇcek, M. Marek, Meso-scale modelling of CO oxidation in digitally reconstructed porous catalyst, Chem. Eng. Sci. 61 (10) (2006) 3240–3249. [45] P. Koˇcí, M. Isoz, M. Plach´ a, A. Arvajov´ a, M. V´ aclavík, M. Svoboda, E. Price, V. Nov´ ak, D. Thompsett, 3D reconstruction and pore-scale modeling of coated catalytic filters for automotive exhaust gas aftertreatment, Catal. Today 320 (2019) 165–174. ˇ ep´ [46] P. Koˇcí, F. Stˇ anek, M. Kubíˇcek, M. Marek, Modelling of micro/nano-scale concentration and temperature gradients in porous supported catalysts, Chem. Eng. Sci. 62 (18-20) (2007) 5380–5385. ˇ ep´ [47] P. Koˇcí, V. Nov´ ak, F. Stˇ anek, M. Marek, M. Kubíˇcek, Multi-scale modelling of reaction and transport in porous catalysts, Chemical Engineering Science 65 (1) (2010) 412–419. [48] M. Dud´ ak, V. Nov´ ak, P. Koˇcí, M. Marek, P. Blanco-García, G. Jones, Prediction of diffusivity and conversion of n-decane and CO in coated Pt/γ-Al2O3 catalyst depending on porous layer morphology, Appl. Catal. B 150-151 (2014) 446–458. [49] M.H. Allouche, R. Enjalbert, F. Alberini, M. Ariane, A. Alexiadis, Development of a combined solver to model transport and chemical reactions in catalytic wall-flow filters, Chem. Eng. Res. Des. 117 (2017) 681–687. [50] K. Yamamoto, M. Nakamura, H. Yane, H. Yamashita, Simulation on catalytic reaction in diesel particulate filter, Catal. Today 153 (3-4) (2010) 118–124. [51] K. Yamamoto, K. Yamauchi, Numerical simulation of continuously regenerating diesel particulate filter, Proc. Combust. Inst. 34 (2) (2013) 3083–3090. [52] K. Yamamoto, T. Sakai, Simulation of continuously regenerating trap with catalyzed DPF, Catal. Today 242 (2015) 357–362. [53] C. Karakaya, P.J. Weddle, J.M. Blasi, D.R. Diercks, R.J. Kee, Modeling reaction–diffusion processes within catalyst washcoats: I. Microscale processes based on three-dimensional reconstructions, Chem. Eng. Sci. 145 (2016) 299–307. [54] Hekmatzadeh A, Keshavarzi H, Talebbeydokhti N, Torabi Haghighi A. Lattice Boltzmann solution of advection-dominated mass transport problem: a comparison. Scientia Iranica. 2018. [55] Krüger T, Kusumaatmaja H, Kuzmin A, Shardt O, Silva G, Viggen EM. The Lattice Boltzmann: Method Principles and Practice: Springer International Publishing; 2017. XXIV, 694 p. [56] D. Vidal, C. Ridgway, G. Pianet, J. Schoelkopf, R. Roy, F. Bertrand, Effect of particle size distribution and packing compression on fluid permeability as predicted by lattice-Boltzmann simulations, Comput. Chem. Eng. 33 (1) (2009) 256–266. [57] J. Ohser, F. Mücklich, Statistical Analysis of Microstructures in Materials Science, Wiley and Sons (2000) 115 p. [58] C.L.Y. Yeong, S. Torquato, Reconstructing random media. II. Three-dimensional media from two-dimensional cuts, Phys. Rev. E 58 (1) (1998) 224–233. [59] C.L.Y. Yeong, S. Torquato, Reconstructing random media, Phys. Rev. E 57 (1) (1998) 495–506. [60] F.A.L. Dullien, in: Porous Media, Elsevier, 1979, pp. 75–155. [61] D. Vidal, R. Roy, F. Bertrand, On improving the performance of large parallel lattice Boltzmann flow simulations in heterogeneous porous media, Comput. Fluids 39 (2) (2010) 324–337.

18

Copyright © 2020 COEK.INFO. All rights reserved.